The motion of a screw dislocation in response to the applied shear stresses shown in Fig.7.2b . the direction of movement is perpendicular to the stress direction.
For an edge, motion is parallel to the shear stress. However, the net plastic deformation for the motion of both dislocation types is the same.
The direction of motion of the mixed dislocation line is neither perpendicular nor parallel to the applied stress, but lies somewhere in between.
Fig.7.2 The formation of a step on the surface of a crystal by the motion of (a) an edge dislocation and (b) a screw dislocation. Note that for an edge, the dislocation line move in the direction of the applied shear stress τ ; for a screw, the dislocation line motion is perpendicular to the stress direction.
Dislocation density --------the number of dislocation in a material is expressed as the total dislocation length per unit volume, or equivalently, the number of dislocations that intersect a unit area of a random section.
The units of dislocation density are millimeters of dislocation per cubic millimeter or just per square millimeter.
When metals are plastically deformed, some fraction of the deformation energy (approximately 5% ) is retained internally, the remainder is dissipated (lost 消失 ) as heat. The major portion of this stored energy is as strain energy associated with dislocations.
Lattice strains (Fig.7.4) --- some atomic lattice distortion exists around the dislocation line because of the presence of the extra half-plane of atoms.
Fig.7.4 Regions of compression (dark) and tension (colored) located around an edge dislocation.
The strains extend into the surrounding atoms, and their magnitudes decrease with radial distance from the dislocation.
The strain fields surrounding dislocations in close proximity to one another may interact such that forces are imposed on each dislocation by the combined interactions of all its neighboring dislocations. ( Fig.7.5)
Fig.7.5 (a) Two edge dislocation of the same sign and lying on the same slip plane exert a repulsive force on each other; C and T denote compression and tensile regions, respectively. (b) Edge dislocations of opposite sign and lying on the same slip plane exert an attractive force on each other. Upon meeting, they annihilate each other and leave a region of perfect crystal.
slip system - ------ This combination of the slip plane and the slip direction. The slip system depends on the crystal structure of the metal and is such that the atomic distortion that accompanies the motion of a dislocation is a minimum.
For a particular crystal structure, the slip plane is that plane having the most dense atomic packing, that is has the greatest planar density.
5. Plastic deformation of polycrystalline metals
For polycrystalline metals, the direction of slip system varies from one grain to another. For each, dislocation motion occurs along the slip system that has the most favorable orientation (i.e., the highest shear stress). ( Fig. 7.10 )
Gross plastic deformation of a polycrystalline specimen corresponds to the comparable distortion of the individual grains by means of slip. (Fig. 7.11)
During deformation, mechanical integrity and coherency are maintained along the grain boundaries. As a consequence, each individual grain is constrained, to some degree, in the shape it may assume by its neighboring grains.
Polycrystalline metals are stronger than their single-crystal equivalents, which means that greater stresses are required to initiate slip and the attendant yielding.
Macroscopic plastic deformation corresponds to the motion of large numbers of dislocations, the ability of a metal to plastically deform depends on the ability of dislocations to move.
Restriction or hindering dislocation motion renders a material harder and stronger.
The size of the grains, or average grain diameter, in a polycrystalline metal influences the mechanical properties. (Fig. 7.14)
Fig.7.14 The motion of a dislocation as it encounters a grain boundary, illustrating how the boundary acts as a barrier to continued slip. Slip planes are discontinuous and change directions across the boundary.
The grain boundary acts as a barrier to dislocation motion for two reasons
Since the two grains are of different orientations, a dislocation passing into grain B will have to change its direction of motion; this becomes more difficult as the crystallographic misorientation increases.
The atomic disorder within a grain boundary region will result in a discontinuity of slip planes form one grain into the other
Alloys are stronger than pure metals because impurity atoms that go into solid solution ordinarily impose lattice strains on the surrounding host atoms.
Lattice strain filed interactions between dislocations and these impurity atoms result, and consequently, dislocation movement is restricted. Fig. 7.16 7.17, 7.18
3. strain hardening or work hardening or cold working ( 形变强化，冷作硬化）
Strain hardening is the phenomenon whereby a ductile metal becomes harder and stronger as it is plastically deformed.
Sometimes it is also called work hardening, or, because the temperature at which deformation takes place is ‘‘cold’’ relative to the absolute melting temperature of the metal, cold working. Most metals strain harden at room temperature.
It is sometimes convenient to express the degree of plastic deformation as percent cold work rather than as strain. Percent cold work (%CW) is defined as
where A 0 is the original area of the cross section that experiences deformation, and A d is the area after deformation.
ductility for copper-nickel alloys, showing strengthening.
Fig.7.17 (a) Representation of tensile lattice strains imposed on host atoms by a smaller substitutional impurity atom. (b) Possible locations of smaller impurity atoms relative to an edge dislocation such that there is partial cancellation of impurity-dislocation lattice strains.
Fig.7.18 (a) Representation of compressive strains imposed on host atoms by a larger substitutional impurity atom. (b) Possible locations of larger impurity atoms relative to an edge dislocation such that there is partial cancellation of impurity-dislocation lattice strains.
Some fraction of the energy expanded in deformations is stored in the metal as strain energy which is associated with tensile, compressive and shear zones around the newly created dislocations. These properties and structures may revert (return) back to the precold-worked states by appropriate heat treatment.
Such restoration results from two different processes that occur at elevated temperatures: recovery and recrystallization, which may be followed by grain growth.
During recovery, some of the stored internal strain energy is relieved by virtue of dislocation motion (in the absence of an externally applied stress), as a result of enhanced atomic diffusion at the elevated temperature.
There is some reduction in the number of dislocations, and dislocation configurations (similar to that shown in Figure 5.12) are produced having low strain energies.
In addition, physical properties such as electrical and thermal conductivities and the like are recovered to their precold-worked states.
Recrystallization is the formation of a new set of strain-free and equiaxed grains that have low dislocation densities and are characteristic of the pre-cold-worked condition. (Fig. 7.21)
After recrystallization, the metal becomes softer, weaker, yet more ductile.
Recrystallization temperature ----the temperature at which recrystallization just reaches completion in 1h. Typically, it is between one third and one half of the absolute melting temperature of a metal or alloy and depends on several factors, including the amount of prior cold work and purity of the alloy.
Fig.7.22 The influence of annealing temperature on the tensile strength and ductility of a brass alloy. Grain size as a function of annealing temperature is indicated. Grain structures during recovery, recrystallization, and grain growth stages are shown schematically.
On a microscopic level, plastic deformation of metals corresponds to the motion of dislocations in response to an externally applied a hear stress, a process termed slip. Slip occurs on specific crystallographic planes and within these planes only in certain directions.
A slip system represents a slip plane- slip direction combination, and operable lips systems depend on the crystal structure of the material.
Grain boundaries serve as barriers to dislocation motion; thus refine the grain size of a polycrystalline metal renders it harder and stronger.
Solid solution strengthening results from lattice strain interactions between impurity atoms and dislocations.
And, finally, as a metal is plastically deformed, the dislocation density increase, as does also the extent of repulsive dislocation-dislocation strain field interactions; strain hardening is just the enhancement of strength with increased plastic deformation .